# Ground state and low-energy excitations of the Kitaev-Heisenberg ladder

←

**Page content transcription**

If your browser does not render page correctly, please read the page content below

Ground state and low-energy excitations of the Kitaev-Heisenberg ladder Cliò Efthimia Agrapidis,1 Jeroen van den Brink,1, 2, 3 and Satoshi Nishimoto1, 2 1 Institute for Theoretical Solid State Physics, IFW Dresden, 01069 Dresden, Germany 2 Department of Physics, Technical University Dresden, 01069 Dresden, Germany 3 Department of Physics, Washington University, St. Louis, MO 63130, USA (Dated: February 4, 2019) We study the ground state and low-lying excited states of the Kitaev-Heisenberg model on a ladder geometry using the density matrix renormalization group and Lanczos exact diagonalization methods. The Kitaev and Heisenberg interactions are parametrized as K = sin φ and J = cos φ with an angle parameter φ. Based on the results for several types of order parameters, excitation gaps, and entanglement spectra, the φ-dependent ground-state phase diagram is determined. Remarkably, the phase diagram is quite similar to that of the Kitaev- arXiv:1902.00466v1 [cond-mat.str-el] 1 Feb 2019 Heisenberg model on a honeycomb lattice, exhibiting the same long-range ordered states, namely rung-singlet (analog to Néel in 3D), zigzag, ferromagnetic, and stripy; and the presence of Kitaev spin liquids around the exactly solvable Kitaev points φ = ±π/2. We also calculate the expectation value of a plaquette operator corresponding to a π-flux state in order to establish how the Kitaev spin liquid extends away from the φ = ±π/2. Furthermore, we determine the dynamical spin structure factor and discuss the effect of the Kitaev interaction on the spin-triplet dispersion. I. INTRODUCTION Though the original KSL was introduced on the honey- comb lattice, it is known that the Kitaev interaction on any 3- Quantum spin liquids (QSLs) have been widely investi- coordinated lattice gives rise to non-trivial properties: In this gated in the last decades. In particular, the introduction of sense, while a one-dimensional (1D) KH chain represented the Kitaev model and related spin liquid, so-called “Kitaev in Fig. 1(a) cannot possess a KSL state, the KH model on a spin liquid (KSL)”, in 20061 has attracted great interest in ladder (we simply refer to it as the KH ladder hereafter) in the condensed matter community. The Kitaev model con- Fig. 1(b) already meets the geometrical requirement. The KH sists of Ising bond-direction dependent interactions (leading ladder can be also extracted from a brickwall lattice [Fig. 1(c) to an exchange frustration) on a honeycomb lattice. Amaz- ], which is geometrically equivalent to the honeycomb lattice: ingly, it is exactly solvable. Few years later, Jackeli and Khal- Cutting along the grey line and folding the cut z-bonds toward liulin pointed out that a strong spin-orbit coupling in the d5 the center we recover the KH ladder in Fig. 1(b). There- transition metal compounds could bring the realization of this fore, it is expected that one can gain insight about the ba- model2 . However, it is not simple to experimentally stabilise sic properties of the honeycomb-lattice KH model from the the KSL because even small amount of Heisenberg interaction KH ladder. In fact, we previously found a certain similar- present in real materials easily takes the system into a mag- ity in magnetic ordering even between the 1D KH model and netically long range ordered (LRO) state. A model containing the honeycomb-lattice KH model15 . Since the interplay of Kitaev and (nearest-neighbor) Heisenberg interactions is the Kitaev and Heisenberg interactions in 2D or 3D geometries so-called Kitaev-Heisenberg (KH) Hamiltonian. The inter- may pose serious challenges to the available numerical meth- play of these two interactions leads to non-integrable ground ods, it is a good strategy to consider the ladder system next. states and requires numerical methods in order to determine We can make use of he density-matrix renormalization group the magnetic properties of the low-energy states. (DMRG) technique to study quasi-1D systems with great ac- In the last decade, a growing number of investigations have curacy16 . Moreover, the ground-state properties and phase been carried out on Kitaev materials3 . Generally, the can- diagram of the coupled KH chains are yet to be extensively didates are classified broadly into two groups in terms of discussed17 . the geometries: Two-dimensional (2D) honeycomb materi- Motivated by this situation, we study the KH ladder us- als such as α-RuCl3 4–6 , Na2 IrO3 , β-Li2 IrO3 7–10 and three- ing the DMRG method in this paper. We obtain the ground- dimensional (3D) hyperhoneycomb materials such as α- and state phase diagram to be composed of four magnetically γ-Li2 IrO3 11,12 . Nonetheless, all these materials exhibit mag- ordered phases, namely rung-singlet, stripy, ferromagnetic netic ordering at low temperature under normal pressures13,14 . (FM)-xy, zigzag; and two liquid phases, namely antiferro- Mostly, further interactions beyond the pure KH model, such magnetic (AFM) KSL and FM KSL, depending on the ra- as long range Heisenberg and off-diagonal exchange interac- tio between Kitaev and Heisenberg interactions. To deter- tions, seem to play a crucial role in the magnetic properties. mine the phase boundaries, we compute several order parame- Recently, the possibility of a pressure and/or field induced ters, excitation gap, and entanglement spectra. Strikingly, the spin liquid state has been also intensively studied. For this rea- phase diagram of the KH ladder is very similar to that of the son, testing a wide variety of internal and external parameters honeycomb-lattice KH model. We then proceed at analyzing on the Kitaev materials has been a subject of active research. the low-lying excitations of the KH ladder by calculating the To evaluate the effect of such parameters correctly, a detailed dynamical spin structure factor with using the Lanczos exact understanding of the pure KH model is becoming more and diagonalization (ED). It is interesting that most of the spectral more important in the context of QSL research. features can be explained by considering those of the 1D KH

2 (a) α where Si,j is the α-component of spin- 21 operator S~i,j at rung i and leg j (= 1, 2), L is the system length, and K and J are (b) the Kitaev and Heisenberg interactions, respectively. The first two lines denote the intra-leg interactions and the last line de- notes the inter-leg interactions: Each leg has a period of two lattice spacing and there are three kinds of bond-dependent interactions. As shown in Fig. 1(c) one finds that the KH lad- (c) der (1) is a system cut out of the KH model on a Brickwall lattice. Since the Brickwall-lattice KH model is obtained by deforming the honeycomb-lattice KH model, the KH ladder is geometrically equivalent to the honeycomb-lattice KH model. Note that the KH ladder has a strong cluster anisotropy, i.e., the periodicity along the z bond is short. Nonetheless, the LRO states observed in the honeycomb-lattice KH model also have a short periodicity in the bond direction and all of them FIG. 1. (a) Lattice structure of the KH chain. (b) Lattice structure of can be reproduced in the KH ladder as shown below. In this the KH ladder studied in this paper. (c) Structure of the KH model paper, to compare magnetic properties of the KH ladder to on a brickwall lattice, which is geometrically equivalent to the hon- those of the honeycomb-lattice KH model, we focus on the eycomb lattice. The grey rectangle shows a cutout that makes the case of equal Kitaev and Heisenberg terms on the three bonds. mapping to the ladder represented in (b) possible. The indices x, y For convenience, we introduce an angle parameter φ, setting and z indicate the three different bonds: x-bond, y-bond, and z-bond, J = cos φ and K = sin φ. respectively. The Hamiltonian (1) can be rewritten as 2 L 2J + K X X + − − + model . 15 Hleg = (Si,j Si+1,j + Si,j Si+1,j ) 4 j=1 i=1 The paper is organized as follows: Our Hamiltonian of the 2 L KH ladder is explained and the applied numerical methods K XX + + − − are described in Sec. II. In Sec. III we present the four kinds + (−1)(i+j) (Si,j Si+1,j + Si,j Si+1,j ) 4 j=1 i=1 of LRO magnetic state that are present depending on the ra- tio between Kitaev and Heisenberg interactions. In Sec. IV 2 X X L z z we discuss the properties of KSL states expanded around the +J Si,j Si+1,j , (2) large limit of Kitaev interaction. In Sec. V the ground states j=1 i=1 are summarized as a phase diagram as a function of the ratio between Kitaev and Heisenberg interactions. We also com- for the intra-leg couplings, and pare the ground-state phase diagram with those of 1D KH L L model and 2D honeycomb-lattice KH model, and discuss the JX + − − + X z z Hrung = (Si,1 Si,2 + Si,1 Si,2 ) + (J + K) Si,1 Si,2 similarity and dissimilarity among them. Sec. VI explains 2 i=1 i=1 the fundamental features of dynamical spin structure factor in (3) each the phase. Finally we conclude in Sec. VII. for the inter-leg, i.e., rung, couplings. We can easily notice that all the nearest-neighbor bonds have a XXZ-type inter- II. MODEL AND METHOD actions, and the sign-alternating double-spin-flip fluctuations acts only along the leg direction. A. Model B. Method We study the KH ladder as represented in Fig. 1(b). The Hamiltonian is described by We employ the DMRG method to investigate the ground- state properties of our model (1). We study finite-size sys- L/2 X L X tems with length up to L × 2 = 160 × 2 with keeping up to x x y y ~i,1 · S ~i+1,1 H=K (S2i−1,1 S2i,1 + S2i,1 S2i+1,1 )+J S m = 4000 density-matrix eigenstates in the renormalization i=1 i=1 procedure. In this way, the truncation error, i.e. the discarded L/2 X L X weight, is ∼ 10−11 . The calculated quantities are extrapo- x x y y ~i,2 · S ~i+1,2 lated to the limit m → ∞ if needed. This allows us to per- +K (S2i,2 S2i+1,2 + S2i−1,2 S2i,2 )+J S i=1 i=1 form very accurate finite-size scaling analysis. We use open L X L X and periodic boundary conditions depending on the quantity +K z Si,1 z Si,2 +J ~i,1 · S S ~i,2 , (1) we consider. To identify the ground state for the given an- i=1 i=1 gle parameter φ, we compute several order parameters, spin

3 gap, plaquette operator, dynamical spin structure factor and (a) entanglement spectra. When we calculate the order parameter under open boundary conditions, the LRO state is observed as a state with a broken translational or spin symmetry. There (b) are in fact several degenerate ground states; one configuration of the degenerate states is selected as the ground state by the initial condition of the DMRG calculation. For the dynamical calculations, we use the Lanczos ED method. To examine the low-energy excitations for each phase, we calculate the dynamical spin structure factor, de- fined as 1 1 Sγ (q, ω) = Imhψ0 |(Sqγ )† Sqγ |ψ0 i π Ĥ + ω − E0 − iη X = |hψν |Sqγ |ψ0 i|2 δ(ω − Eν + E0 ), (4) ν where γ is z or −(+), |ψν i and Eν are the ν-th eingenstate and the eigenenergy of the system, respectively (ν = 0 corre- (c) sponds to the ground state). Under periodic boundary condi- tions, the spin operators Sqγ can be precisely defined by r 2X γ Sqγ = S exp(iqri,j ) (5) L i i,j where ri,j is the position of site (i, j). The sum runs over either i even or i odd sites with fixing j = 1 or 2. They pro- vide the same results. The momentum is taken as q = 4π L n L (n = 0, ±1, . . . , ± 4 ) since the lattice unit cell includes four sites and the number of unit cells is L2 in a system with L × 2 sites. We calculate both spectral functions S± (q, ω) and Sz (q, ω) as they are different due to broken SU(2) symmetry except at φ = 0 and π. We study ladders with L × 2 = 12 × 2, namely, 6 unit cells, by the Lanczos ED method. As shown FIG. 2. (a) Schematic spin configuration of the stripy state. (b) Fi- below, our model (1) contains only commensurate phases with nite size scaling of the stripy order parameter for several values of unit cell containing one, two, or four sites. Therefore, a quan- φ. The dotted line helps the eye follow the data points, solid lines titative discussion for the low-lying excitations is possible represent the linear fitting. (c) Extrapolated stripy order parameter as even within the 12 × 2 ladder. a function of φ/π. III. ORDERED PHASES A. Stripy phase (1.57π < φ < 1.7π) In this section, we present the DMRG results for LRO phases in the ground state. We find four kinds of ordering, Let us start with the stripy state. In the region of 23 π < ∼φ< 7 namely: stripy, rung-singlet, zigzag, and FM-xy phases. The 4 π, since J > 0 and J + K < 0, the leg and rung interac- rung-singlet state is not magnetically ordered but the system tions are AFM and FM, respectively. Thus, we naively expect is in a unique state with dimer ordering, namely, the dimer- the coupled chains to order in what we call the stripy state, as dimer correlation is long ranged. The names of the ordered depicted in Fig. 2(a). Getting back to the original Brickwall phases follow Ref. 8. In the LRO states, except for the rung- lattice, the alignments of up spins and down spins appear al- singlet state, the translational or spin rotation symmetry is bro- ternately with running along the leg. This state can be analyt- ken in a finite system due to Friedel oscillations under open ically proven at φ = tan−1 (−2) ≈ 1.65π, where our model boundary conditions, so that the ordered state can be directly (1) is exactly solvable: The rung Hamiltonian (3) leads sim- observed with a local quantity by extracting one of the degen- ply to isotropic FM couplings due to J + K = −J; whereas, erate states. Generally, the Friedel oscillations in the center of the leg Hamiltonian (2) is reduced to a sum of double-spin-flip the system decay as a function of the system length. If the am- (S + S + +S − S − ) and Ising (S z S z ) parts because the exchange plitude at the center of the system persists for arbitrary system (S + S − + S − S + ) term disappears due to 2J + K = 0. The lengths, it corresponds to a long range ordering. total energy of our system (1) is minimized by taking the wave

4 function as (a) L/2 L/2 1 Y − − Y + + |Ψ0 i = √ S2i,1 S2i,2 | ⇑i + S2i,1 S2i,2 | ⇓i , (6) 2 i=1 i=1 (b) where | ⇑i and | ⇓i denote configurations including only up and down spins, respectively. Note that all the spins are aligned along the z-direction. When the Hamiltonian (1) is applied to this wave function (6), only the Ising terms provide nonzero components. Thus, no quantum fluctuations exist and the system is in a perfect stripy state described by Eq. (6). The ground state energy is E0 /L = 34 J. It is still a nontrivial question how the wave function (6) is modified with moving away from φ ≈ 1.65π. To study it numerically, we introduce an order parameter defined by 1 z z Ostripy (L) = |hS(L/2,1) i − hS(L/2+1,1) i 2 z z (c) +hS(L/2,2) i − hSL/2+1,2) i| (7) Ostripy = lim Ostripy (L) (8) L→∞ In Fig. 2(b), we show finite-size scaling analysis of Ostripy . We see how finite-size scaling is of fundamental importance in this system: the dotted line shows the jump in the order pa- rameter between the smallest (20 × 2) and the second smallest (40×2) systems. The finite size scaling is then performed with discarding the first point, where the system size is too small to stabilize the ordering. This explicitly indicates the existence of “critical length” for stabilizing a long range order. Example of this kind of behavior are seen also for order parameters of the other ordered states. The L → ∞ extrapolated value of the stripy order parameter is plotted in Fig. 2(c). The validity of the exact wave function (6) is confirmed by Ostripy = 1 at φ ≈ 1.65π. Even away from φ ≈ 1.65π, Ostripy keeps rel- FIG. 3. (a) Schematic spin configuration of the zigzag state. (b) Fi- atively large value (∼ 1) and drops down to zero at the both nite size scaling of the zigzag order parameter for several values of φ. edges, φ ≈ 1.57π and φ = 1.7π. It means that the transitions Dotted lines help the eye follow the data points, solid lines represent at both phase boundaries are of the first order. the linear fitting. Note that for φ = 0.53π the order parameters is In our previous paper15 we found that the 1D KH model finite only for L ≥ 140. (c) Extrapolated zigzag order parameter as exhibits a Neél-z state, i.e., Neél ordering with spins parallel a function of φ/π. or antiparallel to the z-axis, for 1.65π 0, ity of zigzag ordering: the leg and rung interactions are FM and AFM, respectively. Hence, an ordered state as in Fig. 3(a) is expected. We call it 1 z z zigzag state by following the name of the corresponding state Ozigzag (L) = |hS(L/2,1) i + hS(L/2+1,1) i 2 in the honeycomb-lattice KH model8 (our straight leg corre- z z sponds to a zigzag line in the honeycomb lattice). Through a −hS(L/2,2) i − hSL/2+1,2) i| (10) similar analysis of the exact wave function (6) at φ ≈ 1.65π, Ozigzag = lim Ozigzag (L) (11) we could assume the wave function at φ ≈ 0.65π to be L→∞ Fig. 3(b)(c) show the finite-size scaling analysis of Ozigzag (L) "L L # 1 Y − Y + |Ψ0 i ≈ √ Si,1 | ⇑i + Si,1 | ⇓i . (9) for several values of φ. At the lower boundary with the AFM 2 i=1 i=1 KSL phase (φ = 0.53π), the long range order settles only at

5 large system sizes L ≥ 140: This can be interpreted as some (a) kind of ”fragility“ of the zigzag ordering close to the AFM KSL. Moreover, it underlines the importance of studying large enough ladders using the DMRG method for this system. In (b) Fig. 3(c) we plot the extrapolated values of Ozigzag in the ther- modynamic limit. We can see that Ozigzag keeps ∼ 0.7 − 0.8 in most of the zigzag phase and Eq. (9) gives a good approx- imation for this zigzag state. Around the lower phase bound- ary (φ ∼ 0.53π), Ozigzag approaches rather continuously to zero with approaching the phase boundary, suggesting a sec- ond order of continuous transition; whereas at the upper phase boundary (φ ∼ 0.8π), Ozigzag drops down to 0, suggesting a first-order transition. For φ < 0.75π, the leading interaction on the rungs is AFM since J + K is positive in Eq. (3). Therefore, the zigzag state may be simply interpreted as antiferromagnetically coupled FM chains (“FM-z state”15 ) obtained in the 1D KH model at 0.65π < φ < π. However, the lower bound of the zigzag phase is significantly more extended (down to φ = 0.53π) (c) than the lower bound of the FM-z state (φ = 0.65π) in the 1D KH model. At 0.5π < φ < 0.65π the 1D KH model is in a liquid state called “spiral-xy state”. Nevertheless, ferro- magnetic fluctuations on the legs would be strong because of the negative J in Eq. (2) and the zigzag ordering can be sta- bilized by the dominant AFM Ising term on the rungs due to J + K > |J| in Eq. (3). In other words, the FM alignment 1 0.8 i-rung on each leg is just taken care of by the interchain AFM cou- 0.6 plings. This may be related to the fragility of the zigzag order 0.4 near the AFM KSL phase. 0.2 0 -0.5 0 0.5 C. Rung-singlet phase (−0.3π ≤ φ ≤ 0.48π) At φ = 0 (J = 1, K = 0), our system (1) is a pure isotropic AFM Heisenberg ladder, known to be in a rung- singlet state with singlet-triplet excitation gap ∆ = 0.5037J FIG. 4. (a) Schematic spin configuration of the rung singlet state, (Ref. 18). The schematic picture of rung-singlet state is given where a red ellipse represents a spin singlet. (b) Finite size scaling of the gap for φ = −0.2π, 0.1π, and 0.47π. (c) Extrapolated spin gap in Fig. 4(a). We compute the excitation gap to see how the as a function of φ/π. Inset: Spin gap of isolated rung as a function perturbation introduced by the Kitaev term affects this state. of φ. Since the total S z is not a good quantum number except at φ = 0, the gap is simply defined as the energy difference be- tween the ground state and first excited state: ∆(L) = E1 (L) − E0 (L) ∆ = lim ∆(L), (12) L→∞ where E0 is the ground state energy and E1 is the first excited scales with the AFM rung interaction. This also means that state energy. Fig. 4(b)(c) show the finite-size scaling analysis the spin-spin correlations are strongly screened. Therefore, a of ∆(L) for several values of φ and the L → ∞ extrapolated single dimer may be expected to be an effective model to re- value of ∆ as a function of φ, respectively. It is remarkable produce the gap behavior. We then extract an isolated rung: that the gap is clearly asymmetric about φ = 0, reaching its J + − − + z z 2 (S1 S2 + S1 S2 ) + (J + K)S1 S2 from our system (1). maximum at φ ∼ 0.1π: this could be understood by noticing This two-site system can be easily diagonalized and the gap is that both K and J are AFM in the region of 0 < φ < 12 ; while, obtained as ∆i−rung = 2J+K 2 for φ < 0 and ∆i−rung = J for K and J have different signs in the region of − 12 π < φ < 0. φ > 0. In the inset of Fig. 4(c) the gap obtained for the iso- The gap closes gradually with approaching the boundary to lated rung is plotted. The qualitative trend the of gap with φ is the stripy phase at φ = −0.3π and to the AFM KSL phase at well described by the single dimer. Furthermore, the gap clos- φ = 0.48π. Thus, they are both continuous transitions. ing points at φ = tan−1 (−2) ≈ −0.35π and φ = 12 π are very Let us provide a more comprehensive explanation about the close to those for the original KH ladder. It proves the strong asymmetry of the gap in respect to φ. In an AFM Heisen- screening of spin-spin correlations in the whole rung-singlet berg ladder, it is known that the magnitude of the gap roughly phase.

6 (a) near the vicinity of φ = π the ground state is approximately denoted by 1 X |ψi ≈ √ |φm i (14) N m where m runs over all the possible spin configurations |φm i z (m = 1 · · · N ) with Stot = 0, ±2, ±4, · · · , ±L, N is the PL number of the spin configurations, i.e., N = n=0 2L C2n = PL (2L)! n=0 (2n)!(2L−2n)! . As a result, the polarized direction is [110] in the spin space, namely, hSix Sjx i = hSiy Sjy i = 18 and hSiz Sjz i = 0 (∀i, j). We call it FM-xy state. This breaking of the SU(2) symmetry is a consequence of the double-spin- (b) flip term, which immediately suppressed the spin polarization along the z-axis. To determine the range of the FM-xy phase, we calculate the total spin per rung S tot /(2L), defined by 2 X L X S tot (S tot + 1) = ~i,j · S S ~i0 ,j 0 (15) j,j 0 =1 i,i0 =1 and the local spin q hSi = x i2 + hS y i2 + hS z i2 hSi,j (16) i,j i,j at the center of the system i = L2 . Note that we can directly detect the local moment in the FM state since the spin rotation symmetry is broken by using open boundary conditions. We FIG. 5. (a) Finite-size scaling of the local spin hSi for several values have confirmed hSi = S tot /(2L) in the thermodynamic limit. of φ. Dotted lines help the eye follow the data points, solid lines Fig. 5 shows 2hSi as a function of φ. At the isotropic SU(2) represent the fitting. (b) Extrapolated values of hSi as a function of point (φ = π), 2hSi = S tot /L = 1. We find that 2hSi decays φ/π. very slowly from 1 as the distance from φ = π, and keeps ∼ 1 in the whole FM-xy region 0.8π < φ < 1.37 < π. The robustness of the FM-xy state is naively expected because D. Ferromagnetic phases both J and J + K are FM at 34 π < φ < 32 π. Then, at both boundaries, to the zigzag state at φ = 0.8π and to the spin At φ = π (J = −1, K = 0), the system is in an SU(2) liquid state φ = 1.37φ, it sharply drops down to 0, which isotropic FM state. This state can be expressed as a sum of indicates first order transitions. fully polarized spin configurations for all of the total S z sec- z = i Siz = 0, ±1, ±2, · · · , ±L. On leav- P tors, namely, Stot ing φ = π, they are lifted: For |π − φ| 1, the first order IV. SPIN LIQUID STATES perturbation in the Hamiltonian (1) is given by 2 L We have determined the phase boundaries of LRO phases 0 π − φ XX + − − + covering most of the φ range. In the remaining two narrow φ H = (S S + Si,j Si+1,j ) 4 j=1 i=1 i,j i+1,j regions around the Kitaev points φ = ± π2 , we found no long 2 L range ordering, i.e., they are spin liquid states. To consider the π − φ XX + + − − similarity to the so-called KSL in the honeycomb KH model, + (−1)(i+j) (Si,j Si+1,j + Si,j Si+1,j ) 4 j=1 i=1 we compute the expectation value of plaquette operator and the excitation gap. L X z z + (π − φ) Si,1 Si,2 , (13) i=1 A. Plaquette operator where the non-perturbative part is the simple FM Heisenberg ladder with J = −1 (∀ nearest neighbor bonds). To gain It is known that the Kitaev model, e.g., on a hexagonal clus- the energy benefits by H0 , the total S z sectors in the wave ter and ladder, is in a π-flux state. This state is characterized z function are restricted to Stot = 0, ±2, ±4, · · · , ±L. Thus, by the expectation value of plaquette operator to be unity. We

7 (a) (a) (b) (b) FIG. 7. (a) Finite-size scaling of the excitation gap as a func- FIG. 6. Expectation value of the plaquette operator around (a) the tion of the inverse system length at the Kitaev points φ = ±π/2. AFM KSL point φ = π/2 and (b) the FM KSL point φ = 3π/2 for (b) Semi-log plot of (a). The blue line is fitting function ∆ = different system lengths. Shaded areas show the neighboring LRO 0.62 exp(−0.52L). phases. The insets in (a) and (b) show the considered 6-site plaquette corresponding to a hexagon in the honeycomb-lattice KH model. honeycomb-lattice KH model. define the expectation value of the plaquette operator for our system (1) as Oplaquette = hS1x S2y S3z S4x S5y S6z i (17) where the numbering of sites is indicated in the inset of Fig. 6. Note that this 6-site plaquette corresponds to a hexagon in the B. Excitation gap honeycomb-lattice KH model. In Fig. 6 we show Oplaquette calculated with ED for several ladder lengths under periodic boundary conditions. The finite-size effect seems to be neg- We compute the excitation gap using Eq. (12) at the two ligible within the spin liquid phases. At both of the Kitaev Kitaev points φ = ±π/2. The results are the same at both points φ = ±π/2, Oplaquette is 1 as expected. With moving points. In Fig. 7(a) the excitation gap is plotted as a function away from φ = ±π/2, Oplaquette decreases but keeps ∼ 1 in of the inverse system size. It seems to indicate a vanishing gap finite regions. In the vicinities of the neighboring LRO phases, in the thermodynamic limit. Actually, as shown in Fig. 7(b) an it decreases rapidly to ∼ 0. This means that the ranges of spin exponential decay is clearly seen by plotting it in a semi-log liquid phases characterized by nonzero Oplaquette are consis- scale. Although this result might seem in opposition with the tent to the phase boundaries with LRO state estimated by order previous studies in Refs. 19 and 20, we can suggest at least parameters and spin moment. Interestingly, the region of FM that no gap exists between the ground state and the first ex- KSL is a few times wider than that of AFM KSL. This is sim- cited state. Within our numerical analyses for the spin liquid ilar to the trend in the honeycomb KH model (see below). We state in the KH ladder we have found no difference from an have also confirmed that the spin-spin correlations are finite isotropic KSL state in the honeycomb-lattice KH model. This only between neighboring sites at the Kitaev points, as in the should be further investigated in future studies.

8 (a) (b) (c) FIG. 8. (a) φ-dependent Phase diagram of the 1D KH model, where Sp-xy, St-xy, and TLL are abbreviations for “spiral-xy”, “staggered-xy”, and Tomonaga-Luttinger liquid, respectively. The details are explained in Ref. 15. (b) Phase diagram of the KH ladder, obtained in this paper. (c) Phase diagram of the honeycomb-lattice KH model21 . rung-singlet gap decreases with increasing the number of KH chains and goes to zero in the honeycomb KH limit. This is essentially the same as the relation between n-leg Heisenberg ladder and 2D Heisenberg model. (ii) The KSL phases in the KH ladder is wider than those in the honeycomb-lattice KH model because the quantum fluc- tuations are stronger due to the low dimensionality. Finally, to get further insights into the topological proper- ties of our system (1), we investigate the entanglement spec- trum22 . Using Schmidt decomposition, the ground state can be expressed as X |ψ = e−ξi /2 |φA B i i ⊗ |φi i, (18) i where the states |φSi i correspond to an orthonormal basis for FIG. 9. Entanglement spectra for representative φ-points of the dif- the subsystem S (either A or B). We study a periodic ladder ferent phases in the ground-state phase diagram. The used system with L × 2 = 32 × 2 sites and divide it into isometric sub- size is L × 2 = 32 × 2 for the LRO states and L × 2 = 24 × 2 for domains A and B with L2 × 2 sites. In our calculations, the the two Kitaev points. ES {ξi } is simply obtained as ξi = − log λi , where {λi } are the eigenvalues of the reduced density matrices after the bi- partite splitting. The low-lying entanglement spectrum levels V. PHASE DIAGRAM are plotted as function of φ in Fig. 9. We find that the lowest level has no degeneracy in the magnetic LRO phases, which are topologically trivial. In the KSL phases, the lowest level Based on the above numerical results, we present the φ- has two-fold degeneracy and of the higher levels have high dependent ground-state phase diagram of the KH ladder in degrees of degeneracy. These are consistent with the ground- Fig. 8(b). For comparison, we also show the ground-state state phase diagram. phase diagrams of the KH model on a single chain15 and on a honeycomb lattice21 in Fig. 8(a) and (c), respectively. In our previous paper15 , we argued that the φ-dependent phase diagram of the 1D KH model is similar to that of the VI. LOW-LYING EXCITATIONS 2D honeycomb-lattice KH model; all the LRO states of the honeycomb-lattice KH model can be interpreted in terms of In this section, we study the low-lying excitations of the the coupled KH chains. In this paper, surprisingly, we found KH ladder by calculating the dynamical spin structure factor. that the phase diagram of just two coupled KH chains, i.e., We compute both S z (q, ω) and S − (q, ω) for each of the LRO the KH ladder, is getting more similar to that of the 2D phase. For the FM KSL state we compute them at three differ- honeycomb-lattice KH model. Only recognizable differences ent φ values to study the effect of the Heisenberg interaction are the followings: on the dispersion. The calculations were done using ED and a (i) The Neél phase is replaced by rung-singlet phase. The ladder of size L = 12 × 2 with periodic boundary conditions.

9 (a) (a) (b) (b) (c) (c) (d) FIG. 11. Dynamical structure factors in the FM KSL phase, calcu- lated with a 12 × 2 ladder under periodic boundary conditions for (a) φ = 1.4π, (b) φ = 1.5π, and (c) φ = 1.54π. The left and right panels show S z (q, ω and S − (q, ω), respectively. The results for the AFM Kitaev point φ = 0.5π are exactly the same as in (b). A. Rung-singlet phase Fig. 10(a) shows the dynamical structure factors for the rung-singlet state at φ = 0.2π (J ∼ 0.81, K ∼ 0.59). FIG. 10. Dynamical structure factors calculated with a 12 × 2 ladder The largest peak appears in S − (q = 0, ω ∼ 0.6) reflecting with periodic boundary conditions in the (a) rung-singlet (φ = 0.2π), the dominant AFM fluctuations along the leg. The value of (b) stripy (φ = 1.64π), (c) zigzag (φ = 0.6π), and (d) FM-xy (φ = ω ∼ 0.6 corresponds to the excitation gap ∆ estimated above. 0.9π) phases. The left and right panels show S z (q, ω and S − (q, ω), The intensities in S − (q, ω) are larger than those in S z (q, ω) respectively. The red dotted lines are guide to the eye and red solid lines are spin-triplet dispersion obtained by the spin-wave theory.

10 due to the easy-plane xy anisotropy. As indicated in dotted D. FM states line, the spin-triplet dispersion ω(q) of S z (q, ω) can be well explained by that of the 2-leg Heisenberg ladder with the ra- Fig. 10(d) shows the dynamical structure factors for the tio between rung and leg interactions rung leg ≈ J+K J ∼ 1.7 FM-xy state at φ = 0.9π(J ∼ −0.95, K ∼ 0.30). The largest − (Ref. 23). The spin-triplet dispersion of S (q, ω) is simi- peak in S − (q = 0, ω ∼ 0) confirms that the spins lie mostly lar in shape but it splits with the width ∼ ± K 2 at q = π. on the xy-plane. The other features are very similar between This splitting of spin-triplet dispersion is a general feature in S z (q, ω) and S − (q, ω). Both of them have the same excitation system including the sign-alternating double-spin-flip term15 . dispersion as The width of spin-triplet dispersion in S z (q, ω) and S − (q, ω) roughly scales to J and J + K 2 , respectively. 2J + K q ω1 (q) = − 1 ± cos , (20) 2 2 and B. Stripy phase 2J + K q ω2 (q) = − 1 ± cos + 2|K|. (21) 2 2 Fig. 10(b) shows the dynamical structure factors for the The splitting between ω1 (q) and ω2 (q) becomes zero in the stripy state at φ = 1.64π (J ∼ 0.43, K ∼ −0.9) where isotropic SU(2) summetric point at q = π and it is roughly the single leg can be basically regarded as an easy-axis AFM proportional to |K|. XXZ Heisenberg chain. In S z (q, ω) the largest peak appears at (q, ω) = (0, 0) due to the Neél ordering along the leg. Very few weights in the other momenta prove the validity of Eq. (6) with almost perfect alignment of spins parallel or antiparallel E. Kitaev spin liquid to z-axis and very weak quantum fluctuations. Whereas, the spin-triplet dispersion of S − (q, ω) is basically explained by In Fig. 11 we show the dynamical structure factors around a single magnon dispersion. Thus, the spectral weight is al- the FM Kitaev point (φ = 32 π). At the FM Kitaev point, most uniform for all q values, and the dispersion is obtained both S z (q, ω) and S − (q, ω) show no dependence on q. This by spin-wave theory as dispersionless feature is a natural consequence of no spin- spin correlations except the nearest-neighbor ones. The dis- K q tance between the lower and upper bound of the continuum in ω(q) = J ± sin . (19) S − (q, ω) is of the order of |K|, relating to the spinon prop- 2 2 agation along the leg. Note that the spectra at the AFM Ki- taev point are exactly the same as those at the FM Kitaev The good agreement can be seen in Fig. 10(b). Since the stripy point. Let us then see the effect of the Heisenberg term on order parameter drops on both phase boundaries, Eq. (19) the spectra. Fig. 11(a) and (c) show the dynamical structure would give at least qualitatively a good approximation for the factors at φ = 1.4π and φ = 1.54π, respectively. Although spin-triplet dispersion in the whole stripy phase. they are almost equally close to the boundary to the neigh- boring phase, the spectra are apparently quite different: At φ = 1.54 it mostly keeps the spectral features at the Kitaev point except that the main peak splits into two peaks with a C. Zigzag phase small interval ∼ J; while at φ = 1.4π the dispersionless fea- ture is completely collapsed and its lower bound looks rather similar to the spin-triplet dispersion of the FM-xy state. It Fig. 10(c) shows the dynamical structure factors for the may be related to the fact that the expectation value of the zigzag state at φ = 0.6π(J ∼ −0.31, K ∼ 0.95) where each plaquette operator deviates faster from the pure KSL value leg is ferromagnetically ordered. The system can be under- (Oplaquette = 1) at φ < 32 π (J < 0) than at φ < 32 π (J > 0) stood as two FM chains coupled by the Ising-like AFM cou- with leaving from the FM Kitaev point. pling. The largest peak in S z (q = 0, ω ∼ 0) reflects the FM ordering along the leg. The weights in the other momenta are small since the spins are mostly aligned along the z-axis; how- ever, they seem to be larger than those for the stripy state. This VII. CONCLUSION implies that the zigzag ordering is more fragile than the stripy ordering. In S − (q, ω) a largest and lowest-lying peak appears We studied the ground state and low-lying excitations of at q = π, indicating a four-site periodicity along the leg. The the KH model on a ladder using the DMRG and Lanczos ED shape of the dispersion is similar to that of the staggered-xy methods. Based on the results of several order parameters, ordered state in the 1D KH model. Nevertheless, the gapped excitation gap, and entanglement spectra, we determined the peak position ω ∼ 0.42 clearly suggests no ordering on the ground-state phase diagram as a function of the ratio between xy-plane. The intensities in S − (q, ω) are larger than those in Kitaev and Heisenberg interactions. It is very rich and in- S z (q, ω) due to the easy-plane xy anisotropy. cludes four magnetically ordered phases such as rung-singlet,

11 stripy, zigzag, FM, and two spin liquid phases. The phase di- finite excitation gap in the rung-singlet phase around φ = 0 agram is strikingly similar to that of the KH model on a hon- due to strong cluster anisotropy, the gap decreases with in- eycomb lattice. Distinct differences are only the presence of creasing the number of legs and becomes zero in the limit of a rung-singlet phase instead of the Néel state and a few times 2D honeycomb-lattice KH model. We also calculated the dy- wider ranges of two spin liquid phases. These differences can namical spin structure factor using the Lanczos ED method. be understood by the dimensionality: (i) Since the quantum Interestingly, most of the spectral features in the KH ladder fluctuations are typically stronger in a lower dimensional sys- can be explained by considering those of the 1D KH model. tem, it is more difficult to stabilize LRO state in the ladder Note added — During the preparation of this manuscript, than in a 2D system. (ii) Though the 2-leg KH ladder has a we became aware of Ref. 24. Their phase diagram agrees very well with ours. 1 A. Kitaev, Annals of Physics 321, 2 (2006). A. Al-Zein, M. M. Sala, M. Krisch, J. Chaloupka, G. Jackeli, 2 G. Jackeli and G. Khaliullin, Physical Review Letters 102 (2009), G. Khaliullin, and B. J. Kim, Nature Physics 11, 462 (2015). 11 10.1103/physrevlett.102.017205. V. M. Katukuri, R. Yadav, L. Hozoi, S. Nishimoto, and J. van den 3 S. Trebst, arXiv preprint arXiv:1701.07056 (2017). Brink, Scientific Reports 6 (2016), 10.1038/srep29585. 4 12 A. Banerjee, C. A. Bridges, J.-Q. Yan, A. A. Aczel, L. Li, M. B. B. Huang, W. Choi, Y. B. Kim, and Y.-M. Lu, Physical Review B Stone, G. E. Granroth, M. D. Lumsden, Y. Yiu, J. Knolle, S. Bhat- 97 (2018), 10.1103/physrevb.97.195141. 13 tacharjee, D. L. Kovrizhin, R. Moessner, D. A. Tennant, D. G. Y. Singh and P. Gegenwart, Physical Review B 82 (2010), Mandrus, and S. E. Nagler, Nature Materials 15, 733 (2016). 10.1103/physrevb.82.064412. 5 14 S.-H. Do, S.-Y. Park, J. Yoshitake, J. Nasu, Y. Motome, Y. S. R. D. Johnson, S. C. Williams, A. A. Haghighirad, J. Singleton, Kwon, D. T. Adroja, D. J. Voneshen, K. Kim, T.-H. Jang, J.-H. V. Zapf, P. Manuel, I. I. Mazin, Y. Li, H. O. Jeschke, R. Va- Park, K.-Y. Choi, and S. Ji, Nature Physics 13, 1079 (2017). lentı́, and R. Coldea, Physical Review B 92 (2015), 10.1103/phys- 6 R. Hentrich, A. U. Wolter, X. Zotos, W. Brenig, D. Nowak, revb.92.235119. 15 A. Isaeva, T. Doert, A. Banerjee, P. Lampen-Kelley, D. G. C. E. Agrapidis, J. van den Brink, and S. Nishimoto, Scientific Mandrus, S. E. Nagler, J. Sears, Y.-J. Kim, B. Büchner, and Reports 8 (2018), 10.1038/s41598-018-19960-4. 16 C. Hess, Physical Review Letters 120 (2018), 10.1103/phys- S. R. White, Physical review letters 69, 2863 (1992). 17 revlett.120.117204. A. Metavitsiadis, C. Psaroudaki, and W. Brenig, 7 Y. Singh, S. Manni, J. Reuther, T. Berlijn, R. Thomale, W. Ku, arXiv:1806.02344 [cond-mat] (2018), arXiv: 1806.02344. 18 S. Trebst, and P. Gegenwart, Physical Review Letters 108 (2012), S. R. White, R. M. Noack, and D. J. Scalapino, Phys. Rev. Lett. 10.1103/physrevlett.108.127203. 73, 886 (1994). 8 19 S. K. Choi, R. Coldea, A. N. Kolmogorov, T. Lancaster, I. I. N. Wu, Physics Letters A 376, 3530 (2012). 20 Mazin, S. J. Blundell, P. G. Radaelli, Y. Singh, P. Gegenwart, K. R. X.-Y. Feng, G.-M. Zhang, and T. Xiang, Physical Review Letters Choi, S.-W. Cheong, P. J. Baker, C. Stock, and J. Taylor, Physical 98 (2007), 10.1103/physrevlett.98.087204. 21 Review Letters 108 (2012), 10.1103/physrevlett.108.127204. J. c. v. Chaloupka, G. Jackeli, and G. Khaliullin, Phys. Rev. Lett. 9 T. Takayama, A. Kato, R. Dinnebier, J. Nuss, H. Kono, L. Veiga, 110, 097204 (2013). 22 G. Fabbris, D. Haskel, and H. Takagi, Physical Review Letters H. Li and F. D. M. Haldane, Phys. Rev. Lett. 101, 010504 (2008). 23 114 (2015), 10.1103/physrevlett.114.077202. T. Barnes, E. Dagotto, J. Riera, and E. S. Swanson, Phys. Rev. B 10 S. H. Chun, J.-W. Kim, J. Kim, H. Zheng, C. C. Stoumpos, C. D. 47, 3196 (1993). 24 Malliakas, J. F. Mitchell, K. Mehlawat, Y. Singh, Y. Choi, T. Gog, A. Catuneanu, E. S. Sørensen, and H.-Y. Kee, arXiv preprint arXiv:1812.04003 (2018).

You can also read